JOURNAL OF IMAGING SCIENCE AND .TECHNOLOGY • Volume 41, Number 2, March/Apri11997
Drying of WaterBased Inks on Plain Paper* M. Sami Selim, Victor F. Yesavage, Rachid Chebbi, and Seung H. Sung Colorado School of Mines, Golden. Colorado 80401
Jens Borch and John M. Olsont Lexmark International, Boulder. Colorado 80301
Previous studies in inkjet printing have considered ink penetration into paper or ink evaporation to be effective in the drying process. In the present study, a unified approach that allows for simultaneous evaporation and penetration during the drying process was applied. To this end, penetration rates were measured experimentally using a Bristow tester. In addition, evaporation rates were determined from a theoretical evaporation model that contained no adjustable parameters. It was found that for plain paper used in the office environment, the rate of penetration was at least 20 x higher than the rate of evaporation. Accordingly, ink drying is determined mainly by penetration, and penetra· tion curves alone are sufficient to predict the dry time or ink disappearanj:e on a plain paper surface. In practice, this is illustrated by inkjet print quality on plain papers of various sizing treatments. The sizing level needs to be adjusted according to the desired inkjet image. That is, fullcolor printing requires penetration rates sufficient 'to accommodate each of the process inks applied without color bleed or other inktoink interaction processes. This may be at expense of character and line print deterioration due to fiber swelling in monocolor printing. Journal of Imaging Science and Technology
152158 (1997)
Introduction In spite of recent advances in inkjet paper manufacture 1 spurred by the rapid growth in lowend color printers, a detailed understanding of the ink drying process is still lacking. This is particularly so for the plain paper types used in the office environment. Generally, these are treated with chemicals that provide water resistance to the paper (sizing treatments). While this is beneficial to the general end usage of these papers, it also may provide a tremendous variation in print quality for inkjet printing depending on ink formulation and printer design. The complexity of the paper structure, both physically and chemically, provides several ways in which a waterbased ink may penetrate.2 For inkjet drops impacting the paper surface at relatively high speeds, analysis has been restricted to mainly visual observation of dried drop sizes 3 or quantita
Original manuscript received October 16, 1996.
t IS&T Member • Presented in part at the 46th Annual Conference of IS&T, the Society for Imaging Science and Technology, Cambridge, MA, May 914, 1993 and at the 47th Annual Conference of IS&T, Rochester, NY, May 1520, 1994.
© 1997, IS&TThe Society for Imaging Science and Technology
152
tive measurements using video analysis. 2 For larger liquid volumes, quantitative penetration measurements can be carried out more readily, using, for example, the Bristow test procedure. 1 The Bristow tester is a useful tool for comparing the liquid uptake of different plain papers but, so fa r, it has not been shown to simulate the inkjet printing process fo r the much smaller ink drop volumes. Most studies in inkjet printing have emphasized the ink penetration into paper as being the main mechanism for drying without considering the additional effect of ink evaporation. In contrast, one studyfi has treated ink evaporation as the main controlling drying step. Another study 2 has considered evaporation as being too slow to contribute to the drying process. In the present approach simultaneous evaporation and penetration will be considered. Penetration measurements will be based on Bristow test analysis.
Theory Our goal is to develop a mathematical model that can be used to predict the drying rate of a waterbased ink film deposited on a paper surface. To this end, we first develop an evaporation model that can be applied to calculate the rate of drying under the assumption that drying takes place due to evaporation alone. The model, which is free from any adjustable parameters, is developed for a pure liquid evaporating in a quiescent atmosphere under isothermal conditions. Evaporation rates calculated from this model provide the maximum evaporation rate possible for a waterbased ink film under quiescent conditions. Next, we· present a model that can be used to calculate the penetration rate of ink into paper. The penetration model is based on the LucasWashburn equation that requires knowledge of the absorption coefficient. The latter can be determined experimentally; for example, using a Bristow tester. Finally, we use results from both models to arrive at a combined model that allows for ink drying under simultaneous evaporation and penetration into the paper. Evaporation Model. Consider a waterbased ink film of initial height Z 0 and initial temperature T _ as shown in Fig. 1. Water evaporates from the flat ink surface into a vapor region that extends an infinite distance above the ink surface. The vapor consists of the diffusant A (water vapor) and a gas B (air) that is insoluble in the liquid film . The initial concentration of A, PAo• and the initial temperature, T_, in the gas phase are both uniform. At any timet, the ink film occupies the region 0 < z < Z(t) and the air occupies the region Z(t) < z < oo, where Z(t) denotes the position of the evaporating interface. The desire is to find an expression for the location of the inkair interface Z (t) as a function oftime t.
Evaporation
t t t t t
Ink Film
z 0.1
Paper Substrate
~
1
+ Penetration 0 .01
Figure 1. Waterbased ink film evaporating from and penetrating into a paper substrate.
To seek an analytical solution to the problem, we assume an ink film consisting of pure liquid water and neglect any temperature variation during the evaporation process. Thus, we consider the evaporation of a pure liquid under isothermal conditions. Under these conditions, • the solution will provide an upper bound for the evaporation rate of a waterbased ink on paper. This is because the lowering of the liquid temperature due to evaporation or the addition of glycol to the ink will result in a lowering of the water vapor pressure at the inkair interface and hence the evaporation rate. With these assumptions, the process will be conirolled by mass diffusion of the evaporating species (water vapor) through the vapor phase. Accordingly, the appropriate equations governing the mass concentration, PA• of the water vapor through the vapor region may be written as:
()pA +(1Pr..JdZ ()pA =D ()2pA AB at2 ' Pu dt ()z at
Z(t)<z<= {1) '
subject to the following initial and boundary conditions:
t = 0,
{2)
Z 0 < z < = , t = 0,
(3)
Z = Z(t), t > 0,
(4)
J
(5)
dZ, opA _ ( 1 PA,eq D ABPL  dt Pu iJz
Z = Z(t), t > 0,
z too, t > 0.
(6)
In Eq. 1, Pv denotes the mass density of the vapor phase, PL denotes the mass density of the liquid phase, and DAB is the diffusion coefficient of A in B. The quantity PA.•q in Eqs. 4 and 5 represents the gasphase concentration of A at the moving interface. For the case of isothermal evaporation of a pure liquid, PA.eq is constant. Equations 1 through 6 are readily solved using similarity transformations with the similarity variable 11 = 2~ D ABt . The final solution is given by
erfcl zZo (1PLJA,l Pu ~4DABt
O.Q1
0 .1
Figure 2. Graph based on Eq. 10 for determining the evaporation parameter A.. (8)
dZ dt
=A. ~ DAB t
(9)
'
where A. is the root of the following transcendental equation:
P.l:._;.J erfc(Pr.. t.Jexp(Pr.. ( Pu Pu Pu
;.J
2
= __1_ P.1.cq
P 110.
.JTC Pu  PA.cq
( 10)
Equation 7 gives the concentration distribution of water vapor in the gas phase as a function of z and t , Eq. 8 gives the location of the evaporation front as a function of time, and Eq. 9 gives the velocity of the evaporation front. The root A. of Eq. 10 may be interpreted as the dimensionless location of the evaporation front, [Z(t) Z 0 ] I ~4DABt, and also as the dimensionless evaporation front velocity, (dZ I dt) I~ D ABt. The solution of Eq. 10 for A. is readily determined using the NewtonRaphson method 6 and is presented in Fig. 2. Note that the abscissa in this figure is not the group appearing on the right of Eq. 10. The abscissa in this figure is a more convenient group in practice and is related to the group on the right side of Eq. 10 as follows:
PA,eq PAo Pv PAo PA ,eq PAo = _PA ,eqPAo Pv PA,eq 1 Pv PAo
(11)
Using regression analysis, numerical results from the solution of Eq. 10 were used to develop the following explicit equations for A.: In A.*= 0.5247 + 1.0091ln p*, for 0.001 < p* < 0.1, (12)
(7)
Drying of WaterBased Inks on Plain Paper
0 .001 0 .001
In A.*= 0.1771 + 2.1679ln p* + 0.7016[ln p*J2 + 0.1449[ln p*]3, for 0.1 < p* < 1.0,
(13)
Vol. 41, No. 2, March/April1997
153
where
). * =_ p L
).
and p* = p A ,eq
Pv

p AO
Pv PAo
(14)
For a waterbased ink evaporating under TAPPI conditions of 23°C and 50% RH, we find Pv = 1.194 kg/m3 , PL = 1000 kg/m 3 , PAo =0.01027 kg/m 3 , andpA,eq =0.02054 kg/m3 • With these values, Eq. 12 gives A =5.86
X
(15)
106
Taking the diffusivity of water vapor in air at 23°C as 2.6 x 104 J.1 2lms, Eq. 9 gives the evaporation rate as 9.45x 104
{i
Jlm 1 ms.
(16)
The minus sign in this equation indicates that Z(t) decreases with time. Note that the z axis is taken positive in the upward direction. Penetration Model. The penetration of an ink film into pa per is readily obtained from the LucasWashburn equation7 if a hydrophobic liquid is applied. For more hydrophilic liquids , such as waterbased ink films, the penetration mode is more complex.8•9 Penetration may be faster due to fiber swelling and capillary expansion or slower due to saturation ofliquid into capillaries. 9•10 Additionally, the process is affected by the specific interaction between the liquid and the surface chemistry of the paper fibers in the surface structure. 11 Based on this and Bristow penetration analysis of water penetration into paper structures including plain printing papers,9 we propose to use the following equation fot the penetration rate of an ink film into paper: (17) where Vis the volume ofliquid absorbed into the paper in ml/m2 , tis the time in ms, K, is the roughness index in mll m 2 , and K. is the absorption coefficient in ml!(m 2·msm). Because a thickness of 1 Jlm is equivalent to a volume of 1 ml/m2 , Eq. 17 also may be written as (18) where K, is now in Jlm and K. in Jlm/msm. Note that the numerical values of K, and K. are identical. Differentiating Eq. 18 with respect to time, we obtain the penetration rate as: = mKatmlJlm I ms. ( dZ) dt pent
(19)
Note that a minus sign has been inserted on the right side of Eq. 19 because the film thickness decreases with time as penetration occurs. Combined Evaporation and Penetration Model. We now consider ink film drying by evaporation and penetration. Because both processes occur simultaneously, a mass balance on the ink film gives (20) Substituting for the evaporation and penetration rates from Eqs. 9 and 19, we obtain
154
Journal of Imaging Science and Technology
Wetting Delay
tw (Contact Time) 0·5 , (ms)o.s Figure 3. Bristow plot describing the liquid uptake versus square root of time.
dZ) ( dt
=). ~ DAB t
_ mK tm1. a
(21)
Integration of this equation gives the following expression for the variation of the film thickness with time: (22)
For the values of A. and DAB given above, Eqs. 21 and 22 become
(~~)=
9.45 x 104
{i
(23) (24)
Experimental Using Eq. 23 for the ink film thickness decrease or Eq. 24 for the ink film thickness at different times requires the measurement of K. and m via plots like that shown in Fig. 3 where m = 0.5. Using mixtures of ethylene glycol and water, this was carried out for two copy paper brands; one typical of the acidmade rosinsized paper used for xerographic copying and laser printing and the other typical of the alkalinemade syntheticsized paper now being substituted for the acidmade paper grade in mill conversions.12 Figures 4 and 5 show the liquid volume uptake variations on a squareroot time basis (m = 0.5). For the rosinsized paper (Fig. 4), K. varied from 0.11 to 0.27 depending on the ethylene glycol content. For the syntheticsized paper (Fig. 5), liquid uptake was much more rapid and could not be measured for ethylene glycol concentrations higher than 20% because of complete penetration of the relatively thin (.. 100 !J.m) 20lb paper base. Additionally, it is apparent that squareroot time linearity is not followed for the syntheticsized paper brand. The liquid uptake on a squareroot time basis is not linear but may be brought to a linear basis by assuming a higher exponent of time (m = 0.9) as shown in Fig. 6. In this case K. varied from 0.025 to 0.044.
Selim et al.
16

•
60wt% EG
D
50wt%EG
•
40 wt% EG
0
D.W.
"'E
g o
25
10%EG D.W. 20%EG

+ 30wt% EG
::::.
.s
20
"C
C"
•
:.J
.c ....
• •
t:.
"'E
12
·:; "C <D
. ._
. 30
10wt%EG
C"
:.J 20wt% EG
10
·:; "C <D
en
.c ....
<(
.c
0
0
.c
15
en
<(
8
10 6+r~~~
0
10
20
30
5+r~~~~~
(Contact Time) 0 S, (ms) 0 ·s
0
100
300
400
(Contact Time) 0·9 , (ms)o.9
Figure 4. Liquid uptake versus square root of time for rosinsized paper. 30.~
200
Figure 6. Liquid uptake for syntheticsized paper on linear basis (m = 0.9).
• 20%EG A D.W. 9
• 10% EG
25
EVAPORATION ONLY
8
"'E
g
7
20
'E
"C
E,
·:;
C"
:.J
' N
15
"C <D
6
5 4
.c .... 0
en
.c <(
3
10
2
5 0 o+~~r~~~r~
0
5
10
15
20
25
30
(Contact Time) 0 ·5 , (ms)o.s Figure 5. Liquid uptake versus square root of time for syntheticsized paper.
Results
Evaporation versus Penetration. Form = 0.5 in Eq. 24 and the K. values found for the rosinsized paper (the least penetrating paper), it is apparent that the film thickness loss due to evaporation is of the order of 1% of that due to penetration. Lower values forK. have been reported
Drying of WaterBased Inks on Plain Paper
2
3
4 .[t,
5
6
7
8
9
10
(sec )0·5
Figure 7. Calculated film thickness variation with time for a 10~mthick film drying by evaporation alone and by penetration with absorption coefficients K. = 0.01, 0.05, and 0.11.
in the literature, 13 but still at these levels, the thickness loss due to penetration is about 20 times larger than the corresponding loss due to evaporation. Lower penetration rates are possible for papers by adding more sizing (hardsized papers), changing the chemical nature of the sizing, or varying the filler or paper structure. However, this creates drying rates that are unacceptably high for inkjet printing. This is seen from calculated results presented in
Vol. 41, No.2, March/April1997
155
Figure 8. Color r eproduction of fullcolor print quali ty on paper similar to tha t tested in Fig. 4.
Figure 9. Color reproduction of fullcolor print quality on paper similar to that tested in Figs. 5 and 6.
156
.Journ a l o[Jmaging Science a nd Technology
Selim et al.
Fig. 7, where the film loss due to drying of a 10!!mthick film is compared to drying at different penetration levels and to drying due to evaporation alone. ForK" levels below 0.11, the drying time increases beyond 10 s. The even slower drying by evaporation alone agrees with the experimental findings of Oliver, Agbezuge, and Woodcock,~ for drying ofinkjet drops on non penetrating mylar material. For evaporation to play a role in inkjet drying one must increase the proportionality factor defined by A. beyond the value (0.0019) given in Eq. 24. This can be done through ink formulation (nonwaterbased inks) or by heat assistance. Several inkjet printers have been marketed relying on the latter principle. Discussion Print Quality. To test the results obtained using the modeling approach and Bristow testing with glycol water mixtures, fullcolor printing was carried out on various copy papers using an IBM ColorJetprinter PS 4079.* This printer prints with composite inks of relatively low glycol content (z20%) at a relatively high speed requiring rapid ink drying. All printing was carried out under TAPPI environmental conditions (TAPPI T402) such that evaporation rates should be very similar for all of the papers tested and similar to that assumed in the theoretical calculation. Yet, print quality varied greatly as seen in Fig. 8 for an acidmade rosinsized paper similar to the one quantified by Bristow testing and in Fig. 9 for one like the alkalinemade syntheticsized paper also studied by Bristow testing. The rosinsized paper exhibited graininess due to color bleed in fullcolor areas but superior character and line definition for singlecolor printing. The syntheticsized sheet showed much better print definition in fullcolor areas but at the expense of more raggedness for character and line print
Figure 10. Singledot images on paper similar to that tested in Fig. 4.
Drying of WaterBased Inks on Plain Paper
ing. We believe that this behavior simulates the penetration characteristics defined by Bristow testing. The higher penetration rate for the syntheticsized sheet results in drying the ink amounts applied in fullcolor printing by transferring individual colors from the sheet surface before another is applied. The lower penetration rate for the rosinsized sheet creates a situation where colors bleed together before drying. Because differences in evaporation rates were not created, the difference in print quality must be solely due to penetration. The deterioration in character and line printing for slacksized paper is well known for lower resolution blackonwhite inkjet printers."Âˇ 14 For the 4079 printer, this difference is less pronounced but becomes visible in singledot printing as shown in Figs. 10 and 11. Dot fuzziness in the alkalinemade paper (Fig. 11) may be interpreted as created by ink penetration into fiber cell walls and lumens immediately after inkpaper contact as indicated by the instant upward curvature of the Bristow plot in Fig. 5YÂˇ 10 Dot definition is much less dependent on fiber structure in the acidmade paper (Fig. 10). This is due to wetting delay followed by nonswelling penetration (Fig. 4). Here, Bristow testing appears to simulate as pects ofinkjet printing in that sufficient paper sizing prevents penetration into the fiber structure. Note that the paper acidity depends mainly on the filler used and not so much on paper fiber structure or sizing and also that paper acidity by itself is not the major variable in determining print quality. Conclusions â€˘ By comparing evaporation rates calculated using an experimental model wit h penetration rates obtained using Bristow testing, we conclude that drying rates depend on paper penetration in inkjet printing with waterbased inks.
Figure 11. Singledot images on paper similar to that tested in Figs. 5 and 6.
Vol. 41, No. 2, March/April 1997
157
• Because penetration is the functional process in nonheatassisted inkjet printing, paper sizing contributes to inkjet image on plain paper brands. That is, fulleolor printing requires penetration rates sufficient to accommodate each of the process inks applied without color bleed or other inktoink interaction processes. However, this may be at the expense of character and line print deterioration due to fiber swelling in monocolor printing. A • IBM is a registered trademark and Color Jetprinter is a trademark of International Business Machines Corporation in the United States and/ or other countries and used under license.
13.
International Congress on Advances in Non·lmpsct Printing Technolo· gies, Portland, OR, 163 (1991). S. J. Bares, in Handbook of Imaging Materials, A. S. Diamond, Ed., Marcel Dekker, Inc., New York, 1991, pp. 545562. ASTM Standard 0 5455·93. A. Borhan, S. B. Pence, and A H. Sporer, J. lmaging Techno/. 16: 65 (1990). W.S. Darn and D.O. McCracken, Numerical Methods, John Wiley & Sons, Inc. , New York, .1972, pp. 2530. M. B. Lyne, in Handbook of Physical and Mechanical Testing of Paper and Paperboard, 2, R. E. Mark, Ed., Marcel Dekker, Inc., New York, 1984, pp. 103141 . R. W. Hoyland, in FiberWater Interactions in Papsr·Making, F. Bolam, Ed., British Paper and Board Federation, London, 1978, pp. 557577. M. B. Lyne and J. S. Aspler, Tappi 65: 98 (1982) . M. B. Lyne, in Products of Papermaking, 2, C. F. Baker, Ed., Pira International, Leatherhead, U.K., 1993, pp. 885911 . J. Barch, in Products of Papermaking, 1, C. F. Baker, Ed .. Pira International, Leatherhead, U.K., 1993, pp. 209236. J. Barch, TAPPI Short Course Notes, 1990 Neutral/Alkaline Papermaking Short Course, Orlando, FL, 39 (1990) . M. Shimomura, Y. Sato, Y. Suga, and H. Noguchi, J. Imaging Techno/.
14.
S. J. Bares and K. R. Rennels, Tappi J. 73: 123 (1990).
3.
4. 5.
6. 7. 8.
9. 10. 11 .
12.
References 1. 2.
158
D. L. Lee, W. H. Fass. and A.T. Winslow, Advance Printing of Papers, IS& 47th Annual Conference/ICPS 1994, Rochester, NY, 823 (1 !194 ). J. F. Oliver, L. Agbezuge, and K. Woodcock, Proceedings of IS& 7th
rs
rs
16: 189 (1990).